Microscopic Theory of Entropic Bonding for Colloidal Crystal Prediction
Total Page：16
File Type：pdf, Size：1020Kb
Microscopic Theory of Entropic Bonding for Colloidal Crystal Prediction Thi Vo1 and Sharon C. Glotzer,1,2∗ 1Department of Chemical Engineering, University of Michigan – Ann Arbor 2 Biointerfaces Institute, University of Michigan – Ann Arbor ∗To whom correspondence should be addressed; E-mail: [email protected]. Entropy alone can self-assemble hard particles into colloidal crystals of remarkable complexity whose structures are the same as atomic and molecular crystals, but with larger lattice spacings. Although particle-based molecular simulation is a powerful tool for predicting self-assembly by exploring phase space, it is not yet possible to predict colloidal crystal structures a priori from particle shape as we can for atomic crystals based on electronic valency. Here we present such a first principles theory. By directly calculating and minimizing excluded volume within the framework of statistical mechanics, we describe the directional forces that emerge between hard shapes in familiar terms used to describe chemical bonds. Our theory predicts thermodynamically preferred structures for four families of hard polyhedra that match, in every instance, previous simulation results. The success of this first principles approach to entropic colloidal crystal structure prediction furthers fundamental understanding of both entropically driven crystallization and conceptual pictures of bonding in matter. 1 Introduction In his 1704 treatise, Opticks, Sir Isaac Newton wrote of an “attractive” force that holds particles of matter together. By observing that matter stays together in a host of different everyday situations, he inferred the presence of what we now refer to as chemical bonds, one of the most fundamental concepts in science. Chemical bonds originate in electronic interactions. Together with thermodynamics, chemical bonds allow us to predict and understand materials structure and properties, including the way in which atoms arrange to form crystals, from the ionically bonded simple lattice of table salt to the covalently bonded structure of diamond to multicomponent alloys with many thousands of atoms in a unit cell held together by delocalized metallic bonding. Like atoms, nanoparticles can self-assemble under thermodynamic driving forces into crystal structures of extraordinary complexity and diversity (1–6). What “force” would Newton infer from observing these “colloidal” crystals? From his writings, he would undoubtedly infer an attraction – a bond – between particles as for atoms, but of a different origin and at larger length, time, and energy scales. Indeed, DNA linkers, ligand-ligand pairs, protein-antibody pairs, and opposite charges are all examples of bonding elements exploited to self-assemble colloidal crystals of nanoparticles, which effectively serve as “atoms.” But what would Newton make of colloidal crystals self-assembled from hard particles whose only attribute, like billiard balls, is the inability to overlap? Remarkably, many reported hard particle colloidal crystals are isostructural to known atomic crystals with covalent, ionic and metallic bonding (7–13). For example, all 14 Bravais lattice types (7), Frank-Kasper (7), clathrate structures (11), open lattices (14), multiple quasicrystals (7, 8), and crystals with as many as 432 particles in the unit cell (11) self-assemble from disordered fluid phases in computer simulations of hard, otherwise non-interacting polyhedra. Experiments likewise find colloidal crystals of hard particles, though the diversity of structures reported to date has been limited by current challenges in making diverse shapes devoid of any energetic interactions (12, 15, 16). Hard particle crystals – in where there is no 2 potential energy – are stabilized by entropy maximization, which, counterintuitively, is achieved when the ordered crystal has more available microstates than the disordered fluid (17–21). In hard particle systems, no explicit bonding elements are required for crystallization. Instead, entropy maximization leads to the emergence of effective, attractive entropic forces with directionality that arises from particle shape and crowding. This directionality creates local valence and, ultimately, long-range order (22,23). The extent to which the same complexity and diversity of structure is possible from chemical bonding and from entropic “bonding” is unexpected and demonstrates that emergent phenomena such as crystal self- assembly are agnostic to the origin of these bonds, provided the system is subject to the laws of thermodynamics. We assert that if entropic bonds are to be considered a useful construct like chemical bonds, then crystal structure prediction using ab initio methods should be possible, in the same way that atomic crystal structures can be predicted from a knowledge of chemical bonding to solve Schrodinger’s Equation (24,25). Here, we report an ab initio theory of entropic bonding that does not involve computer simulations but instead predicts thermodynamically preferred crystal structures directly from particle shape and a mean-field description of directional entropic forces. Using traditional statistical mechanics, we develop a framework for calculating entropic bonds between arbitrarily shaped particles. We test our theory on several challenging examples to show that our method correctly selects the thermodynamically preferred crystal structures reported in simulations. For brevity, we limit our discussion to single-component crystals composed of hard polyhedral particles, although generalization to multi-component crystals of arbitrarily shaped hard or patchy particles (26, 27) is foreseeable. Lastly, by comparing similarities in mathematical form for our statistical mechanical theory with quantum theory, we posit that theoretical ideas from quantum mechanics might be useful, if only by analogy, for understanding colloidal systems and vice versa. The success of our theory not only provides a new way to predict colloidal self-assembly, but also presents a potentially unifying framework that bridges our understanding of crystallization across different length scales. 3 Results Our theory builds upon two fundamentals tenets of statistical mechanics. First, thermodynamic systems evolve to the most probable state. Second, the probability of any microstate – in this case, a unique arrangement of particles – depends on the energy of that microstate. Consider a system of 푁 hard particles of identical size and shape contained within a fixed volume 푉. Because hard particles don’t interact, there is no energy and thus all microstates are equally probable. The most probable thermodynamic state is then the one with the largest number (훺) of microstates, or, equivalently, the maximum entropy S via Boltzmann’s expression 푆 = 푘퐵 ln 훺 . For hard particle systems, maximizing entropy is equivalent to maximizing all of the empty (so-called “free”) volume into which a new particle can be placed without overlapping another particle (20,21). Maximizing free volume is, in turn, achieved by minimizing the excluded volume around each particle (17,20). In lieu of directly calculating excluded volume (and thus entropy) in our system, we approximate excluded volume using a mathematical ansatz described below. In this way, we obtain an eigenvalue equation whose solution gives the free energy of a colloidal crystal structure without need for thermodynamic integration (34,35), a routine method for free energy calculation that relies on simulation. In what follows, we present the key results in our derivation, and leave the mathematical details to the Supporting Materials (SM). Pseudoparticle Ansatz We propose an ansatz in which all empty space within the system of N hard anisotropic particles in a volume V is filled with 푁푝푃 fictitious pseudoparticles (pP), each of which is much smaller than a particle, can freely overlap each other, and is attracted to anisotropic particles with an interaction energy we derive below. To avoid confusion, we hereafter refer to the anisotropic particles as nanoparticles (NPs), which are not to be confused with the fictitious pPs. In the limit of low NP density, the pP spatial distribution will be roughly uniform. At 4 intermediate and high NP densities, the pP density distribution will become spatially dependent, conforming to the NP shape as the excluded volume becomes more and more spatially heterogeneous. Testing different NP arrangements and selecting for those that optimize the pP density distribution will yield the colloidal crystal structure with the maximum entropy among the set of structures tested. By representing the effective entropic forces by explicit forces between NPs encapsulated in a mean-field pP-NP interaction potential, we will predict the thermodynamically preferred structure that would otherwise necessitate computer experiments using Monte Carlo or molecular dynamics simulation. Interaction Between Nanoparticles and Fictitious Pseudoparticles We perform a self-consistent mean-field approximation (28) in the [푁, 푁푝푃, 푉 , 푇] statistical mechanical ensemble where we integrate over all NPs except for a single reference NP (or pP) to obtain the following pP-NP interaction potential (see Section II of the SM for details), 푁 −2 훽푈(푟) = [ln 푝푃(푟) − 훽휇푝푃]푟 + ∑ 푈푐표푟푒(푟) (1) 푖 where 훽 = 1/푘퐵푇, 푝푃(푟) is the spatially dependent, mean-field density distribution of the pPs, 휇푝푃 is the chemical potential of the pPs, 푈푐표푟푒 represents a hard-core repulsion preventing pPs from overlapping a NP, and r is the distance between a pP